Share this document with a friend

11

Transcript

PHYSICAL REVIEW RESEARCH 2, 033256 (2020)

Valley Zeeman effect and Landau levels in two-dimensional transition metal dichalcogenides

Fengyuan XuanCentre for Advanced 2D Materials and Graphene Research Centre, National University of Singapore,

Block S16, Level 6, 6 Science Drive 2, Singapore 117546

Su Ying Quek*

Department of Physics, Centre for Advanced 2D Materials and Graphene Research Centre,National University of Singapore, 6 Science Drive 2, Singapore 117546, Singapore

(Received 14 February 2020; revised 3 July 2020; accepted 7 July 2020; published 17 August 2020)

This paper presents a theoretical description of both the valley Zeeman effect (g-factors) and Landau levelsin two-dimensional H-phase transition metal dichalcogenides (TMDs) using the Luttinger-Kohn approximationwith spin-orbit coupling. At the valley extrema in TMDs, energy bands split into Landau levels with a Zeemanshift in the presence of a uniform out-of-plane external magnetic field. The Landau level indices are symmetricin the K and K ′ valleys. We develop a numerical approach to compute the single-band g-factors from firstprinciples without the need for a sum over unoccupied bands. Many-body effects are included perturbativelywithin the GW approximation. Nonlocal exchange and correlation self-energy effects in the GW calculationsincrease the magnitude of single-band g-factors compared to those obtained from density functional theory. Ourfirst-principles results give spin- and valley-split Landau levels, in agreement with recent optical experiments.The exciton g-factors deduced in this work are also in good agreement with experiment for the bright and darkexcitons in monolayer WSe2, as well as the lowest-energy bright excitons in MoSe2-WSe2 heterobilayers withdifferent twist angles.

DOI: 10.1103/PhysRevResearch.2.033256

I. INTRODUCTION

When a weak external magnetic field is applied to aperiodic system, there are two physical effects on the bandextrema. First, Bloch states are reorganized into highly degen-erate Landau levels (LLs). Second, LLs are further shifted inenergy, known as the Zeeman effect. In recent years, the semi-nal prediction of spin-valley coupling caused by broken inver-sion symmetry in semiconducting monolayer (ML) H-phasetransition metal dichalcogenides (TMDs) [1] has led to a surgein theoretical and experimental interest in the response ofTMDs to external magnetic fields for valleytronic applications[2–8]. Inversion symmetry breaking and threefold rotationalsymmetry also lead to valley-dependent optical selection rules[1,9–11], which have enabled experimentalists to measure thevalley-dependent Zeeman effect [7] and Landau levels [8] inthese TMDs. Theoretically, how energy band edges at eachvalley respond to the external magnetic field is essential tounderstand both phenomena. However, most theoretical workstarget each effect separately.

Published by the American Physical Society under the terms of theCreative Commons Attribution 4.0 International license. Furtherdistribution of this work must maintain attribution to the author(s)and the published article’s title, journal citation, and DOI.

On the one hand, the band edge Zeeman shift has beenexplained by the band- and valley-dependent orbital magneticmoment mnk, or Laudé g-factor gorb

nk , given by mnk = gorbnk μB.

In Ref. [12], the authors show that Peierls substitution intoa multi-band k · p Hamiltonian matrix results in a term thatis linear in the external magnetic field, which was used todefine the Laudé g-factor. However, the final expressions donot contain information on LLs. Another approach that hasbeen widely used is to define the orbital magnetic momentusing semiclassical considerations [13]. This semiclassicalmethod also does not lead to expressions for LLs. On the otherhand, LLs in TMDs have been derived using the massive Diracfermion model [14–16], obtained by Peierls substitution intoa two-band tight binding (TB) model. This model results inLL indices that are asymmetric between the K and K ′ valleys[14–16], with no Zeeman term.

To explain experiments in which both the valley Zeemaneffect and LLs are important [8,17], one needs to find ageneral approach to take into account the two effects on anequal-footing framework. However, in many cases, the abovetheories are patched together in an ad hoc fashion to interprettransport and optical measurements in the literature [8,17–19]. Specifically, the LLs obtained from the massive Diracfermion model are further shifted by an additive Zeeman term,which is obtained from one of the models that deduced anexpression for the Zeeman term without the LL effect. Sucha simple mixing of different models is not convincing. Oneobjection is from Niu et al., who have suggested that theLLs from the massive Dirac fermion model should not be

2643-1564/2020/2(3)/033256(11) 033256-1 Published by the American Physical Society

FENGYUAN XUAN AND SU YING QUEK PHYSICAL REVIEW RESEARCH 2, 033256 (2020)

further shifted by any Zeeman term [15]. Fundamentally, thisconfusion of how to treat both the Zeeman effect and LLsarises from the fact that the Zeeman effect and LLs have beenexplained separately with different model Hamiltonians. Theuse of different Hamiltonians also leads to controversies in theinterpretation of the g-factors.

Existing quantitative predictions of the single-band g-factor can be summarized into two approaches [5]. The firstapproach is based on a phenomenological model [20], wherethe orbital magnetic moment is partitioned into atomic andvalley terms, so that the total single-band g-factor consistsof three terms, namely, the spin, atomic, and valley terms[2]. Since the valence band maximum (VBM) and conductionband minimum (CBM) of TMDs are composed mainly ofd orbitals, atomic contributions are taken as their magneticquantum numbers ±2 and 0 [21]. The valley term is ap-proximated to be inversely proportional to the effective mass[8,9,22,23]. However, for models with more than two bands,such a relation does not hold anymore [12]. Another problemis that the partitioning of the orbital magnetic moments intoatomic and valley terms has not been justified properly—inparticular, it is not clear whether they are additive and if thereare other contributions left. The second approach is based onPeierls substitution into an effective multiband k · p Hamil-tonian [12], which has been discussed above. Contrary to thephenomelogical model, the authors argue that atomic termsare vanishing and the effect from remote bands is believed tobe important. In a later work, it is shown that Hamiltonianswith different number of bands lead to very different excitong-factors [24]. Although both approaches can give g-factorsin reasonable agreement with experiment, their numerics verymuch depend on the specific model Hamiltonian chosen.

Kormányos et al. have proposed to reduce a multibandk · p Hamiltonian to a single-band model using Löwdin-partitioning [25]. In this case, the energy expressions for theband extrema contain both the Zeeman term and LLs. How-ever, one drawback of this approach is that the g-factor used inthe Zeeman term is model-dependent, and in particular, alsodoes not have the atomic contribution that was suggested inthe phenomelogical models.

In this work, to describe both the valley Zeeman effectand LLs in two-dimensional (2D) TMDs, we propose usinga general Hamiltonian including spin-orbit coupling (SOC)for an electron in a periodic potential perturbed by a uniformexternal magnetic field. Our key results are as follows: withinthe Luttinger-Kohn (LK) approximation [26], the valley bandedges split into LLs with a valley-dependent Zeeman shift. Incontrast to previous predictions [8,12,15,20,25], LL indicesobtained from the present work are symmetric with respectto the K and K ′ valleys, and the orbital magnetic momentdescribing the Zeeman shift is shown to be equivalent tothe compact Berry-curvature-like expression derived usingthe semiclassical approach [13]. We further extend the LKapproximation to electrons in a nonlocal periodic potential,where the compact form of the magnetic moment remainsunchanged. This extension allows us to include nonlocalexchange and correlation effects in our predictions for thesingle-band g-factor, which have not been discussed before.We implement an approach to evaluate the Berry-curvature-like expression for the g-factor without the need for a sum

over unoccupied bands, using first-principles Hamiltonians.We use density functional theory (DFT) as well as many-bodyperturbation theory within the GW approximation, and obtainresults for prototypical TMD systems. First, the single-bandg-factor and Berry curvature obtained using DFT are found tobe quite different from those derived using a TB Hamiltonian[27]. Deriving analytically separate components of the orbitalmagnetic moment using a tight-binding basis, we provideclear definitions of the valley and atomic terms of the orbitalmagnetic moment and furthermore, uncover an additionalcross term, which arises from a coupling between the phasewinding of Bloch states and the parent atomic orbitals. The de-viation of our TB results from DFT originates from the omis-sion of atomic and cross terms. Second, compared to DFT,GW self-energy effects increase the magnitude of single-bandg-factors significantly while keeping exciton g-factors in MLWSe2 approximately unchanged. For the interlayer excitonsin MoSe2-WSe2 heterostructures, GW results for exciton g-factors agree better with experiments than DFT. Finally, thesingle-band g-factors, together with our predictions for the LLspacings, result in spin- and valley-split LLs, consistent withthe optical experiment by Mak et al. [8].

Our theoretical formalism is presented in Sec. II and inAppendices A–C, where treatment of nonlocal potentials isspecifically discussed. Our numerical method is also pre-sented in Sec. II, with numerical results shown and dis-cussed in Sec. III. In Sec. IV, we summarize the paper anddiscuss briefly the possibility of accounting for the energy-dependence of the self-energy. Derivations of the atomic,valley, and cross terms of the orbital magnetic moment areincluded in Appendix D.

II. THEORETICAL APPROACH

A. Formalism

We start with the general Hamiltonian of an electron ina local periodic potential with SOC, in the presence of anexternal magnetic field B = ∇ × A = (0, 0, Bz ):

H = (p + eA)2

2me+ V (r) + HSOC + Hspin,

HSOC = h

4m2ec2

(σ × ∇V ) · (p + eA),

Hspin = gsμB

2σ · B,

(1)

where me is the electron mass, V (r) is the local periodicpotential, μB is the Bohr magneton, and gs ≈ 2 is the free-electron g-factor. σ refers to the Pauli matrices. Because sz isa good quantum number at K and K ′ in the H-phase TMDs [1],the spin-diagonal components of Eq. (1) give the solutions forspin-up and spin-down states. Henceforth, the spin Zeemanterm Hspin is dropped from our equations and will be addedon again in the final result for the energy levels.

We first consider the energy levels of the Hamiltonian ofML TMD without the magnetic field. Using a second-orderexpansion of the energy levels around K , the nondegener-ate quasiparticle energy levels En(K + q) are given by (see

033256-2

VALLEY ZEEMAN EFFECT AND LANDAU LEVELS IN … PHYSICAL REVIEW RESEARCH 2, 033256 (2020)

Appendix A)

EnK+q = EnK + h2q2

2me+ E (2)

nK (q), (2)

where

E (2)nK (q) =

(h

me

)2 ∑m �=n

|〈unK|q · π|umK〉|2EnK − EmK

. (3)

Here, q is the crystal momentum and unK are the periodic partof the Bloch eigenstates of the Hamiltonian without any mag-netic field. Note that if SOC is neglected, π = p + h

4mec2 (σ ×∇V ) is simply replaced by p and all the formalism in whatfollows remains the same. Luttinger and Kohn [26,28] haveshown that if the magnetic field is treated as a perturbation,then, dropping Hspin, the energy levels of the Hamiltonian inEq. (1) can be obtained by solving an effective eigenvalueproblem:

En(K + q)�α = εα�α, (4)

where q in En(K + q) is replaced by the operator q =p/h + eA/h. The effective Hamiltonian En(K + q) requiredin Eq. (4) can then be shown to be

EnK+q = EnK + h2(q2

x + q2y

)2m∗ − mnK · B, (5)

where the effective mass m∗ is

1

m∗ = 1

me+ 1

m2e

∑m �=n

2∣∣�x

nm

∣∣2

EnK − EmK, (6)

with the matrix elements �nm = 〈unK|π|umK〉, and the orbitalmagnetic moment mnK is defined by coefficient of the linearterm on the external magnetic field:

mnK = −iμB

me

∑m �=n

�nm × �mn

EmK − EnK. (7)

Here, we have neglected terms involving qz and �znm as

there is no band dispersion along the z direction in 2Dmaterials. The numerator from Eq. (3) results in a term ofthe form {qx, qy}Re[�x

nm�ymn] + [qx, qy]iIm[�x

nm�ymn]. Using

[qx, qy] = −ieBz/h, Eq. (5) can be readily derived from thethreefold rotational symmetry in TMDs, which gives �x

nm =±i�y

nm [29].Substituting Eq. (5) into Eq. (4), we obtain the equation for

a free electron in the presence of B = (0, 0, Bz ), with energylevels shifted by a term linear in the magnetic field, given by−mnK · B. Thus, solving Eq. (4) and adding on Hspin givesLLs with energies

εN = EnK +(

N + 1

2

)hωc − gorb

nKμBBz + gssz,nKμBBz, (8)

where the cyclotron frequency ωc = eBz/m∗, the quantumnumber α in Eq. (4) is now the LL index N = 0, 1, 2, ..., andthe single-band g-factor is defined as gorb

nKμB = mznK. Notably,

our result shows that the LL indices are symmetric in K andK ′, different from the results obtained from the massive Diracfermion model where the LL indices are valley-dependent[14,15].

We also highlight that the Bloch states are reorganized intoLLs, so that the energies εN depend on the LL indices N , andnot on the crystal momenta, which are not rigorously definedin the presence of an external magnetic field. The orbitalmagnetic moment as defined in Eq. (7) should be evaluatedexactly at the valley extrema. It determines the Zeeman shiftfor all the LLs [Eq. (8)] that are located within the energyrange in which the original Bloch state band structure isquadratic [Eq. (2)].

In contrast to previous work, we do not assume any spe-cific form of the Hamiltonian. Our derivation using the LKapproximation results directly in an energy expression thatincludes both the LLs and Zeeman effects. Compared withthe approach by Kormányos et al. [25] we start from a generalHamiltonian without the need to use a particular multibandk · p model. Thus, the atomic contribution to the magneticmoment in the Zeeman effect is included automatically (seeSecs. II B and III A for more details). Our final expressionfor LLs in Eq. (8) can be directly used to interpret relevantexperiments after obtaining the effective mass and gorb

nK fromfirst principles. The limitation of this approach is that onlyterms up to second order in q are included in the expressionfor energy bands in Eq. (2). So Eq. (8) is only a solution inthe parabolic region of the energy extrema. Applying the LKapproximation to the full band would lead to the Hofstadterbutterfly spectrum [30].

We now discuss another form of Eq. (7). Using the resultfrom perturbation theory that

∂kunk = h

me

∑m

〈umk|π|unk〉Enk − Emk

umk. (9)

mnK in Eq. (7) can be written as

mnK = − ie

2h〈∂kunk| × [Hk − Enk]|∂kunk〉|k=K, (10)

which has the same form as the semiclassical formula for mnKderived in Ref. [13] in the absence of SOC. We emphasizethat Eq. (10) is the orbital magnetic moment of single bandsat nondegenerate band extrema with SOC, which is differentfrom the total orbital magnetic moment that involves summa-tion over all Bloch states [31]. Equation (10) is used instead ofEq. (7) for our calculations of the g-factor, because the formof the orbital magnetic moment in Eq. (10) holds also whenV (r) in Eq. (1) is replaced by a nonlocal potential VNL(r, r′).This is in contrast to the expression in Eq. (7), which requiresthe potential in the Hamiltonian to be local.

In the formalism presented above, we have used the prop-erty of locality in the periodic potential twice. First, in theoriginal proof of the LK approximation, a local periodicpotential V (r) is used in Eq. (1). However, the LK methodcan be approximately extended to the nonlocal case and onemay refer to the discussion in Appendix B. Second, in theexpansion [Eq. (2)] of energy bands in the absence of amagnetic field, the second-order term [Eq. (3)] is valid onlyfor a local potential [see Eq. (A1)]. This means that Eq. (7)is valid only for Hamiltonians with local potentials. For anonlocal potential, we can express this second-order term inthe same form, but with p replaced by a more complicatedexpression, which we call c [32] (see Appendix C for details).From Eq. (3) to Eq. (9), p can be replaced by c and Eq. (10)

033256-3

FENGYUAN XUAN AND SU YING QUEK PHYSICAL REVIEW RESEARCH 2, 033256 (2020)

remains unchanged. Thus, Eq. (10) can directly be used tocompute the g-factors if one were to take into account theeffects of nonlocal many-body corrections to the quasiparticleHamiltonian.

B. Numerical method

In this subsection, we describe our numerical method toevaluate Eq. (10) using first-principles Hamiltonians takinginto account exchange and correlation effects within DFTand within many-body perturbation theory using the GWapproximation.

Our numerical implementation for the DFT g-factors isperformed in the DFT code, QuantumESPRESSO [33]. Theunk in Eq. (10) are obtained as the periodic part of the Blochstates, ψnk = eik·runk, which are the solutions of the Kohn-Sham equations,

HDFTψnk =[

p2

2me+ Vion + VH + Vxc

]ψnk = EDFT

nk ψnk,

(11)

where Vion, VH, and Vxc are the ionic, Hartree, and exchange-correlation potentials. The periodic potential V in Eq. (1) istaken to be the effective mean field potential V MF = Vion +VH + Vxc felt by an electron in the TMD material. For the DFTcalculations in this work, the exchange-correlation functionalis evaluated within the local density approximation (LDA)or the generalized gradient approximation (GGA) using thePerdew-Berke-Ernzerhof (PBE) [34] parametrization. Anyexplicit dependence of the exchange-correlation functional onthe current density [35] is neglected. Similar approximationshave been made for the computation of nuclear magneticresonance chemical shifts, and good agreement with experi-ment was obtained [36]. We use optimized norm-conservingpseudopotentials [37] with an energy cutoff of 60 Ry, and ourground-state charge density is obtained using a 21 × 21 × 1k-grid.

Then the key quantity ∂kunk is calculated as

∂kunk = e−iθ unk+dk − unk

dk, (12)

where eiθ = 〈unk|unk+dk〉/|〈unk|unk+dk〉|. The term eiθ elim-inates the random phase factor between unk and unk+dk,allowing us to use the parallel transport gauge. Since theorbital magnetic moment and Berry curvature are both gauge-independent, such a parallel transport gauge will not affectour numerical results. Thus, we directly evaluate Eq. (10)using the DFT Kohn-Sham Hamiltonian, wave functions andeigenvalues. We have checked the numerical convergence ofboth the Berry curvature and g-factor with respect to themagnitude of dk, which we have taken to be 10−5 timesthe reciprocal lattice constant. Our self-consistent cycle isconverged using an energy criterion of 10−8 Ry. We commentthat the above procedure remains the same whether or notSOC is included in the DFT Hamiltonian.

Although the Kohn-Sham wave functions are typicallya good approximation to the quasiparticle wave func-tions, Kohn-Sham eigenvalues in general cannot be for-mally interpreted as quasiparticle energies. For example, DFT

calculations using LDA and GGA exchange-correlation func-tionals usually underestimate the fundamental gap [38,39].Quasiparticle properties can be formulated rigorously withina Green’s function approach, notably the GW approximationfrom many-body perturbation theory. So, it is important toevaluate the g-factors using the GW Hamiltonian, and weimplement our numerical method in the BerkeleyGW package[40].

DFT calculations are first performed to provide the mean-field starting point for the GW calculation. The GW quasi-particle eigenvalues EQP

nk are then obtained by solving thefollowing equation:

HGWψnk = (HDFT − Vxc + )ψnk = EQPnk ψnk, (13)

where Vxc represents the exchange-correlation potentialpresent in the DFT calculation, = iGW is the GW self-energy approximated by product of the Green’s functionand the screened Coulomb interaction W (r, r′). For the pur-pose of this paper, we ignore the energy dependence in ,using the so-called static Coulomb-hole-screened-exchange(COHSEX) approximation, introduced by Hedin [38,41]. Inthe COHSEX approximation, the self-energy consists of twoterms:

= SEX + COH,

SEX(r, r′) = −occ∑nk

ψnk(r)ψnk(r′)∗W (r, r′),

COH(r, r′) = 1

2δ(r − r′)[W (r, r′) − v(r, r′)].

(14)

SEX is the nonlocal screened-exchange interaction and COH

is the local Coulomb-hole term that represents the effect fromthe rearrangement of electrons around the quasiparticle [38].The dielectric matrix used to evaluate the screened Coulombinteraction is calculated within the random phase approxima-tion.

Since the DFT wave functions are a good approximation tothe quasiparticle wave functions [38], ∂kunk can be obtainedfrom the DFT calculation. To evaluate the orbital magneticmoment, one simply needs to substitute the quasiparticle GWeigenvalues into Enk, and use HGW for the Hamiltonian H inEq. (10):

mnK = − ie

2h〈∂kunk| × [

HGWk − EQP

nk

]|∂kunk〉|k=K.

(15)

GW calculations with spinor wave functions are computation-ally challenging. Given that the electron spin is nearly 100%polarized in the vicinity of each valley in the TMDs [42], wecan evaluate the GW correction to the g-factors using scalarwave functions, and then add these corrections to the g-factorscomputed using two-component spinor wave functions inDFT, thereby including SOC effects into GW g-factors. For allthe GW calculations in this work, we use a cutoff of 35 Ry forthe dielectric matrix and a nonuniform sampling [43] of theBrillouin Zone starting with a 12 × 12 k-grid. Our g-factorsare unchanged when the k-grid is increased to 18 × 18.

033256-4

VALLEY ZEEMAN EFFECT AND LANDAU LEVELS IN … PHYSICAL REVIEW RESEARCH 2, 033256 (2020)

FIG. 1. (a) Top view of ML MoS2. Blue and yellow balls rep-resent Mo and S atoms, respectively; (b) Brillouin zone with highsymmetry k-path; (c) Band structure from DFT-PBE (red lines) anda three-band TB model [27] (black dots), without SOC.

III. NUMERICAL RESULTS AND DISCUSSION

A. DFT versus TB in ML MoS2

We compute the band structure, single-band g-factors, andBerry curvature in ML MoS2, using DFT LDA and PBEcalculations, as well as using a three-band TB model takenfrom Ref. [27]. The atomic structure is shown in Fig. 1(a),where the lattice constant is taken to be the same as thatused in Ref. [27] (3.19 Å). The band structures calculatedusing DFT-PBE and using the three-band TB model [27]agree very well [Fig. 1(c)]. Table I shows our numericalresults for the single-band g-factors and Berry curvature atthe K valley. The three-band TB [27] results obtained in thiswork are consistent with those in Ref. [27]. Our DFT Berrycurvature also agrees very well with DFT calculations in theliterature, which were evaluated using the Kubo formula [44].The good agreement of our results with the literature validate

TABLE I. Single-band g-factors and Berry curvatures (� in Å2)at the K point of ML MoS2 computed using the three-band TB modelfrom Ref. [27] and DFT methods. The subscripts, c and v, refer tofrontier conduction and valence bands, respectively, while ↑ and ↓refer to spin-up and spin-down bands at K .

TB [27] LDA PBE PBE-SOC

gorbc −3.98 −1.94 −1.91 −2.05(↑) −1.83(↓)

gorbv −2.99 −4.18 −4.18 −4.25(↑) −4.05(↓)

�c −17.12 −9.01 −8.82 −9.97(↑) −8.00(↓)

�v 15.82 9.95 9.72 10.90(↑) 8.89(↓)

our numerical approach, and in particular, the use of Eq. (12),which avoids the sum over unoccupied states.

From Table I, we find that the effect of SOC on the g-factors and Berry curvature is small, and roughly the samefor the conduction and valence bands. This is in contrast tothe effect of SOC on the energy levels at the valleys, wherethe SOC splitting in the VBM is one order of magnitudelarger than in the CBM [42]. In the following section, wewill see that the effect of SOC is larger for the g-factors inWSe2. Next, for non-SOC calculations, one can see that boththe g-factors and Berry curvature are almost the same forLDA and PBE, which suggests that at the DFT level, usinglocal or semi-local exchange-correlation functionals makes nodifference in predicting single-band g-factors. However, theresults computed using the three-band TB model [27] andDFT are quite different from one another. Meanwhile, wenotice that in Ref. [45], an 11-band TB model gives 6.0 Å2 for�v , which is different from both the three-band TB model [27]and DFT results. These results strongly indicate that althoughthe TB models [27,45] can reproduce the first-principles bandstructure, it is not reliable for computing the g-factors andBerry curvature.

To obtain physical insight into the origin of the orbitalmagnetic moment (g-factors) and the reason for the differ-ence between first-principles and TB results, we consider atight-binding basis βl = 1√

N

∑R eik·Rφl (r − R) to expand the

Bloch state,

ψnk = eik·runk = 1√N

∑R

eik·RClnkφl (r − R), (16)

where the Einstein summation convention is used. We thenhave

∂kunk = 1√N

∑R

eik·(R−r)∂kClnkφl (r − R)

+ 1√N

∑R

eik·(R−r)i(R − r)Clnkφl (r − R).

(17)

Substitution into Eq. (10) gives three terms (Appendix D),which we call valley (V), atomic (A), and cross (X) terms,

m(V )nk = − ie

2h

[∂kCl ′

nk

]∗ × [Hl ′l − EnkSl ′l ][∂kCl

nk

],

m(A)nk = − e

2me

[Cl ′

nk

]∗Ll ′lC

lnk,

m(X )nk = − e

meIm

{[∂kCl ′

nk

]∗ × �l ′l[Cl

nk

]}.

(18)

The matrix elements are defined as Hl ′l = 〈βl ′ |H |βl〉, Sl ′l =〈βl ′ |βl〉, Ll ′l = 〈βl ′ |r × π|βl〉, �l ′l = 〈βl ′ |π|βl〉. In the above,k is evaluated at K and K′ = −K. If the system has timereversal symmetry, then each term fulfills mnK = −mnK′ . Theexpressions for valley and atomic terms depend, to a largeextent, on the phase winding of the Bloch state and the parentatomic orbital angular momentum, respectively. Thus, theycan be regarded as analytical definitions for the valley andatomic terms used in the literature [20]. The cross term,however, has not been discussed in the evaluation of single-band g-factors. (Note that the atomic term is also similar tothe “local” term in the total orbital magnetization discussed

033256-5

FENGYUAN XUAN AND SU YING QUEK PHYSICAL REVIEW RESEARCH 2, 033256 (2020)

FIG. 2. PBE (red lines) and GW (blue dots) band structure of MLWSe2, with SOC.

in Ref. [46] and a similar cross term also appears in the totalorbital magnetization [46].) A similar result can be obtainedfor the Berry curvature [47]. There, the atomic term vanishesand we have

�nk = i〈∂kunk| × |∂kunk〉 = �Vnk + �X

nk,

�(V )nk = i

[∂kCl ′

nk

]∗ × Sl ′l[∂kCl

nk

],

�(X )nk = 2Re

{[∂kCl ′

nk

]∗ × rl ′l[Cl

nk

]},

(19)

where rl ′l = 〈βl ′ |r|βl〉.In standard TB or multiband k · p Hamiltonian literature,

unk is approximated as Clnk. Thus, the second term in the

expression for ∂kunk [Eq. (17)] is ignored, and only thevalley term is present in the computed g-factors and Berrycurvatures. This explains why the atomic term is missing insome of the previous approaches [15,25,27].

B. DFT versus GW in WSe2 and MoSe2-WSe2

Next, we perform DFT and GW calculations for single-band and exciton g-factors. We choose ML WSe2 as a pro-totypical example of 2H-phase TMDs. Since there is noexperimental data for the lattice constant in ML WSe2, weuse the experimental bulk lattice constant (3.28 Å) for WSe2.Figure 2 shows the PBE and GW band structures for MLWSe2, with SOC effects. One can see that, consistent withGW calculations on similar systems [39], the direct gap at Kis increased by 0.9 eV due to the GW self-energy correction.Table II shows the g-factors from DFT and GW, includingSOC effects. Compared to DFT-PBE, GW increases the mag-nitude of the single-band g-factors significantly. However, ifone were to simply use Eq. (7) for computing the orbitalmagnetic moment, then one would immediately expect thatthe GW g-factors would be smaller in magnitude than theDFT-PBE values, because of the larger GW band gap (Fig. 2).As discussed in Sec. II A, the self-energy correction in theGW approximation is a nonlocal operator, so that one cannotsimply use GW quasiparticle energies in Eq. (7) to com-pute the g-factors, unless the effect of the nonlocal potentialis properly accounted for. The simplest approach is to use

TABLE II. Single-band and exciton g-factors of ML WSe2 byDFT versus GW at K . For the single-band g-factors, c and v refer tothe fronter conduction and valence bands, respectively, while ↑ and↓ refer to spin-up and spin-down bands at K . The superscript “orb”indicates that only the orbital part of the g-factor is given here [seeEq. (8)]. X0 and D0 refer to the lowest-energy bright (spin-allowed)and dark (spin-forbidden) excitons, respectively. The numbers inbrackets include the effects of a frequency-dependent BSE kernel.

gorb PBE GW Experiment

gorbc↑ −2.81 −4.15

gorbc↓ −1.90 −3.24

gorbv↑ −4.86 −6.40

gorbv↓ −4.17 −5.71

gX 0 −4.10 −4.50 −3.7 [12,48] −4.3 [20] −4.37 [7] −4.4 [49]

(gX 0) (−4.26)

gD0 −9.92 −10.32 −9.3 [48] −9.5 [49] −9.9 [29]

(gD0) (−9.76)

Eq. (10), as described in Sec. II, because the compact form ofEq. (10) is unchanged in the presence of a nonlocal potential.The fact that LDA and PBE give rather similar g-factorswhile GW changes the g-factors significantly, shows that thenonlocal exchange and correlation effects in the Hamiltonianand quasiparticle energies [Eq. (10)] play an important role inthe prediction of the single-band g-factors.

We also deduce the exciton g-factors to compare withexperimental results. In the literature, experimentalists havemeasured the exciton Laudé g-factor, gX0, defined as [7,12,20]

�EX0 = EX0(σ+) − EX0(σ−) = gX0μBBz, (20)

where �EX0 is the Zeeman splitting of the first bright neutralexciton (X0) photoluminesence peak in H-phase TMDs in thepresence of an out-of-plane magnetic field Bz. According toour first-principles calculations,

〈ψc,±K|px|ψv,±K〉 = ±i〈ψc,±K|py|ψv,±K〉 (21)

in ML WSe2. Thus, the conduction and valence bands in theK (K ′) valley couple to σ + (σ−) circularly polarized light.From established excitonic physics [39], we know that X0 ishighly localized at the K and K ′ valleys, within the region inwhich the Bloch state band structure is quadratic, allowing usto use Eq. (8) for the energies of the states involved in theX0 exciton. Thus, using the fact that single-particle g-factorsat K and K ′ have the same magnitude but opposite sign,one finds that the bright exciton g-factor gX0 = 2(gorb

v↑ − gorbc↑ ),

and the dark exciton g-factor gD0 = 2(gorbv↑ − gorb

c↓ ) − 4, where−4 comes from spin contributions. Table II lists the brightand dark exciton g-factors derived using the spin-allowed andspin-forbidden transitions. We obtain GW g-factors of −4.50and −10.32 for the lowest energy spin-allowed and spin-forbidden transitions in ML WSe2, respectively. Compared toDFT, although GW increases the absolute value of the single-band g-factors, the DFT and GW exciton g-factors are similarfor this system. One can see that the dark exciton g-factoris slightly larger than gX0 − 4 due to the SOC effect on thesingle-band g-factors. These exciton g-factors, as well as those

033256-6

VALLEY ZEEMAN EFFECT AND LANDAU LEVELS IN … PHYSICAL REVIEW RESEARCH 2, 033256 (2020)

FIG. 3. Energy levels predicted at K and K ′ in ML WSe2 in the presence of a uniform external magnetic field and comparison withexperiment [8]. (a) Horizontal dashed lines denote the energy levels (LLs) obtained using a magnetic field of 9 T. Solid curves represent theenergy bands in the absence of a magnetic field, and dashed curves represent the Zeeman-shifted bands (ignoring LL effects). GW g-factors areused for this plot; a plot using DFT g-factors looks similar. Blue denotes spin-down and red denotes spin-up. (b, c) Predicted energy of bandc1 as a function of magnetic field strength at (b) K and (c) K ′. Solid lines and dashed lines are computed using GW and DFT-PBE g-factors,respectively. (d, e) Magnetic-field dispersion of the LLs of band c1 at the K and K ′ valleys. The vertical axes are the critical electron densitiesrequired to fill the LLs as probed from the onset of Pauli blocking of the corresponding inter-LL optical transitions. This data is obtained fromRef. [8].

obtained from DFT, are in good agreement with experiment(Table II).

The effects of electron-hole interactions on the excitong-factors have been discussed by some authors [50]. Ourconsideration of electron-hole interactions will be publishedseparately [51]. Briefly, we consider the effect of frequency-dependence in the kernel used in the Bethe-Salpeter equation(BSE), and, using a plasmon pole approximation, obtain asmall reduction of the estimated g-factors by about 5.7%. Thisreduction gives exciton g-factors in slightly better agreementwith experiment (Table II).

Using our computed effective masses of 0.32, 0.44 and−0.39 me for the c1, c2 and v1 bands, respectively (seeFig. 3), we predict from first principles the energy levels at thevalleys including both LL and Zeeman effects [Eq. (8)], andour results are shown in Fig. 3. A comparison of Figs. 3(b)and 3(c) with Figs. 3(d) and 3(e) shows that the calculationsare in excellent agreement with experiment (the definitions ofK and K ′ are reversed there [8]). Our results are consistentwith the conclusion in Ref. [8] that the LLs are spin- andvalley-polarized. These energy levels include both the LL andZeeman effects, computed entirely from first principles, andthe g-factors include not only the spin and valley terms, butalso the atomic and cross terms, in contrast to previous work[15,25].

Note that the N = 0 LL in Eq. (8) has a zero-point energyhωc/2, relative to the Bloch state band extrema predicted bytaking into account the Zeeman terms only (see Fig. 3). If wewere to assume that the exciton involves only the VBM andCBM wave functions at K and K ′, then we would obtain anadditional shift in the exciton (photoluminescence) energiesdue to the zero-point energies, which shift the VBM and CBM

values to the LL energies. These terms are independent of thevalley index. However, established excitonic physics showsthat the X0 exciton involves transitions in a small region ofthe Brillouin Zone around K [39]. The degeneracy of eachLL in this region is the number of Bloch states in the originalquadratic band dispersion within an energy range of ±hωc/2from this LL. Meanwhile, the allowed optical transitions arebetween conduction and valence band LLs with the sameindex [52]. Thus, the energies of the states involved in the X0transition are reorganized from the quadratic band dispersionto quantized LL energies, and on average, this reorganizationdoes not shift the exciton energies. The shift in exciton energyat each valley results from the Zeeman terms only. This is alsowhat is observed in experiments [7,12,53] where the shift inexciton energy at K is equal and opposite to that at K ′.

We also compute the g-factor for excitons correspondingto the lowest energy spin-allowed transitions in MoSe2-WSe2

heterobilayers in both AA and AA′ stacking configurations,using the lattice constant in the ML WSe2 calculations. Thesecorrespond, respectively, to twist angles of close to 60◦ and 0◦in Ref. [53] (see Fig. 4). Figure 4 shows a schematic of theinterlayer transitions in MoSe2-WSe2 heterobilayers. For theAA-stacked heterobilayer, the K valley of the WSe2 layer isaligned with the K valley of the MoSe2 layer, and similarlyfor the K ′ valleys. Thus, the valley optical selection rule isthe same as that in the MLs [Eq. (21)]. However, for theAA′-stacked heterobilayer, the K (K ′) valley of WSe2 layer isaligned with K ′(K) valley of MoSe2. Defining the K valley ofthe heterostructure as that for the WSe2 layer, we obtain thefollowing selection rule:

〈ψc,±K|px|ψv,±K〉 = ∓i〈ψc,±K|py|ψv,±K〉, (22)

033256-7

FENGYUAN XUAN AND SU YING QUEK PHYSICAL REVIEW RESEARCH 2, 033256 (2020)

FIG. 4. Schematic figure for interlayer optical transitions in(a) AA and (b) AA′ stacking orders in the MoSe2-WSe2 heterostruc-tures. Blue and red balls represent Mo and W atoms, respectively.Blue and red curves represent the conduction band in MoSe2 layerand valence band in WSe2 layer, respectively. Solid and dashedlines represent spin-up and spin-down states, respectively. The spin-allowed transitions in each valley are labeled by σ+ or σ−, indica-tive of the valley-dependent optical selection rules in these systems.

and as a result, the interlayer exciton g-factor for the AA′-stacked heterobilayer is gX0 = 2(gorb

c↑ − gorbv↑ ).

Table III shows the relevant single-band g-factors, and thededuced exciton g-factors for MoSe2-WSe2 heterobilayers. Itis clear that GW gives interlayer exciton g-factors in betterquantitative agreement with experiment than DFT. This betteragreement is related to the larger magnitude of the single-bandg-factors predicted by GW, underscoring the importance ofincluding many-body effects in the quantitative understandingof the single-band g-factors and exciton g-factors. We notethat interlayer hybridization should be explicitly taken intoaccount to obtain quantitatively accurate exciton g-factors. Ifthe single-band g-factors from isolated MoSe2 and WSe2 MLsare used to deduce the g-factors in the heterobilayer, then theGW exciton g-factors will be −7.14 and 17.92 for AA andAA′-stacked systems. These are larger in magnitude than thevalues calculated directly from the heterostructure.

It is interesting to note that although the definition ofthe K or K ′ valley is arbitrary, the sign of the final excitong-factor is determined once the sign convention of the external

TABLE III. Single-band and interlayer spin-allowed excitong-factors in AA-stacked and AA′-stacked MoSe2-WSe2 bilayers.Atomic symbols in brackets indicate which layer the correspondingband belongs to.

gorb PBE GW Experiment

gorbc↑ (Mo) −1.75 −2.63

AA gorbv↑ (W) −4.84 −6.14gX 0 −6.18 −7.02 6.72 [53]

gorbc↑ (Mo) 1.56 2.43

AA′ gorbv↑ (W) −4.69 −5.81

gX 0 12.50 16.48 −15.79 [53] −15.1 [54]

magnetic field and the light polarization are fixed. The signsof the exciton g-factors we computed for the AA and AA′stackings are opposite to those in experiment [53], where onlythe twist angles were described. In the preparation of thismanuscript, we became aware of Ref. [55] where the authorsshow that shifting the MoSe2 layer to align its Se atom withthe hollow site of the WSe2 layer would change the sign ofinterlayer exciton g-factors. We comment that this is related todifferences in the valley selection rules between the two setsof structures, which originate from the differences in threefoldrotation centers of the two layers [29].

IV. CONCLUSIONS AND OUTLOOK

In conclusion, we have used the Luttinger-Kohn (LK)approximation to provide a unified description of the Zeemaneffect and LLs in 2D TMDs, with both effects being treatedon an equal footing within the same general Hamiltonian. Weextend the original LK approximation to treat a Hamiltonianwith a nonlocal periodic potential, allowing us to take intoaccount nonlocal exchange and correlation effects on thesingle-band g-factors. The resulting energy levels are Landaulevels (LLs) with LL indices that are symmetric in the Kand K ′ valleys. These LLs are shifted by a valley-dependentZeeman term. We develop a numerical approach to computethe Berry curvature and single-particle g-factors at the bandextrema for a general Hamiltonian, without the need for a sumover unoccupied states. Tight-binding (TB), DFT LDA/PBE,and static GW (COHSEX) Hamiltonians are used in our calcu-lations, to illustrate the effect of using increasingly better andmore sophisticated approximations to the quasiparticle Hamil-tonian. The TB Berry curvatures and single-particle g-factorsare very different from the DFT results. This is because theTB results in this work include only the so-called valley terms.However, the inclusion of many-body nonlocal exchange andcorrelation effects within the GW approximation increases themagnitude of the single-band g-factors significantly comparedto DFT. Spin-orbit coupling is included perturbatively. Theresulting LL diagram and exciton g-factors predicted by theGW calculations agree well with experiment, for both MLTMDs as well as twisted heterobilayers. The LLs we predictare spin- and valley-polarized.

An interesting open question is whether it is possible toinclude the energy dependence of the self-energy in the com-putation of the g-factors, using our current theoretical frame-work. In this manuscript, we have limited our considerationsto the static GW approximation. However, one can considerextending the LK approximation to treat an energy-dependentHamiltonian, and include dynamical effects in the GW self-energies. In particular, the fact that our evaluation of thesingle-band g-factor does not require a sum over unoccupiedstates makes such an effort computationally efficient. Theapproach developed here sets the stage for the treatment ofnonlocal energy-dependent self-energy effects on the single-band g-factors and LL energies in TMDs.

Note added. After this manuscript was submitted, a paperon first-principles calculations of exciton g-factors in MLTMDs appeared in the arXiv [56].

033256-8

VALLEY ZEEMAN EFFECT AND LANDAU LEVELS IN … PHYSICAL REVIEW RESEARCH 2, 033256 (2020)

ACKNOWLEDGMENTS

We gratefully acknowledge support from the National Re-search Foundation, Singapore, for funding under the NRFFellowship (Grant No. NRF-NRFF2013-07) and under theNRF medium-sized center programme. Calculations wereperformed on the computational cluster in the Centre forAdvanced 2D Materials and the National SupercomputingCentre, Singapore.

APPENDIX A: SECOND-ORDER EXPANSION OF ENERGYBAND FOR A LOCAL PERIODIC POTENTIAL

In this Appendix, we expand the energy band at a bandextremum point k0. The primary purpose of this Appendix isto lay the groundwork for the discussion in Appendix C andSOC is omitted for simplicity. For a local periodic potential,the single-particle Hamiltonian Hk = e−ik·rHeik·r is

Hk = p2

2me+ V + h

mek · p + h2

2mek2, (A1)

where Hkunk = Enkunk. To find the second-order expansion ofenergy bands about k0, one needs to evaluate

Hk0+q = Hk0 + h

me(hk0 + p) · q + h2

2meq2, (A2)

where q is a small shift relative to k0. Since k0 is a bandextremum, the energy expansion up to second order is

Enk0+q = Enk0 + h2

2meq2 + E (2)

nk0(q), (A3)

where

E (2)nk0

(q) =(

h

me

)2 ∑m �=n

|q · 〈unk0 |p|umk0〉|2Enk0 − Emk0

. (A4)

The coefficient of the linear term in k in Eq. (A1) determinesthe matrix elements in the expression for E (2)

nk0(q) and is

what determines the final expression for the orbital magneticmoment in Eq. (7).

APPENDIX B: LUTTINGER-KOHN APPROXIMATIONFOR NONLOCAL PERIODIC POTENTIAL

In the original proof of the Luttinger-Kohn approximation[28], the wave function in the presence of an external magneticfield B = ∇ × A is represented in a basis of Wannier func-tions WnR(r), which are localized at r = R. (In this Appendix,we adopt the system of units used in Ref. [28].):

ψα (r) =∑

R

�α (R)eieG(R,r)/chWnR(r), (B1)

where

G(R, r) =∫ r

RA(η)dη. (B2)

The proof involves the evaluation of Hψα (r), where H =(p−eA/c)2

2me+ V,

Hψα (r) =∑

R

�α (R)

[(p − eA/c)2

2me+V

]eieG(R,r)/chWnR(r)

=∑

R

�α (R)eieG(R,r)/ch

[p2

2me+ V

]WnR(r). (B3)

In the above equation, the central idea is to move eieG/ch

from the right-hand side of H to its left-hand side, wherethe author used the argument that the Wannier function islocalized at R while the magnetic fields are small and slowlyvarying in comparison to WnR[28]. When one has a nonlocalperiodic potential VNL(r, r′), a similar argument can be used.We need to show that the commutator below is approximatelynegligible:

[VNL(r, r′), eieG(R,r)/ch]WnR(r) ≈ 0. (B4)

The first term of this commutator is∫VNL(r, r′)eieG(R,r′ )/chWnR(r′)dr′

≈ VNL(r, R)WnR(R), (B5)

where we use the fact that G(R, R) = 0 and Wannier orbitalWnR(r′) is localized at R. Next, the second term of thecommutator is

eieG(R,r)/ch∫

VNL(r, r′)WnR(r′)dr′

≈ eieG(R,r)/chVNL(r, R)WnR(R) ≈ VNL(r, R)WnR(R), (B6)

where we further invoke the assumption that the whole for-malism in this work is valid only for weak magnetic fields,for which G(R, r) is small and slowly varying, so that thephase factor eieG(R,r)/ch is also slowly varying compared toVNL(r, R). Thus, the commutator in Eq. (B4) can be droppedapproximately so that the key relation in the original proofholds:

(H + VNL)ψα (r)

=∑

R

�α (R)eieG(R,r)/ch

[p2

2me+ V + VNL

]WnR(r). (B7)

The rest of the proof is not affected by VNL, and in thisway, the Luttinger-Kohn method can be extended, within theapproximation of a weak magnetic field, to treat a nonlocalperiodic potential.

APPENDIX C: SECOND-ORDER EXPANSION OF ENERGYBAND FOR A NONLOCAL POTENTIAL

A general nonlocal potential VNL(r, r′) can be expanded as[32]

VNL(r, r′) = U0(r) + U1(r)r · p + U2(r)(r · p)2 + · · · ,

(C1)

where Ui are all local components. Since VNL(r, r′) doesnot commute with eik·r, there will be an additional termin Hk when there is a nonlocal potential. This term is

033256-9

FENGYUAN XUAN AND SU YING QUEK PHYSICAL REVIEW RESEARCH 2, 033256 (2020)

given by

e−ik·rVNL(r, r′)eik·r = U0(r) + U1(r)r · (p + hk)

+U2(r)[r · (p + hk)]2 + · · · . (C2)

Recall from Appendix A that the term linear in k in Eq. (A1)determines the matrix elements in the expression for E (2)

nk0(q).

In Eq. (C2), there is also a term linear in k, which we cansimply write as k · c. Since all the algebra to derive Eq. (10)in Sec. II A does not depend on the form of c, one can simplyreplace p by c, just as we replaced p with π to include theSOC effect. Therefore, we show that the form of Eq. (10)remains the same when there is a nonlocal potential. However,the momentum matrix in Eq. (7) should be replaced by c toproperly account for the nonlocal potential.

APPENDIX D: PARTITION OF MAGNETIC MOMENT

We provide below a detailed derivation for the partition-ing of the orbital magnetic moment. As in the main text,expanding the Bloch state using a tight-binding basis we have∂kunk = A + B:

A = 1√N

∑R

eik·(R−r)i(R − r)Clnkφl (r − R), (D1)

B = 1√N

∑R

eik·(R−r)∂kClnkφl (r − R). (D2)

Inserting ∂kunk into Eq. (10) we obtain mnk = m(V )nk +

m(X )nk + m(A)

nk .First it is easy to derive the expression for the valley term:

m(V )nk = − ie

2h〈B| × [Hk − Enk]|B〉

= − ie

2h

1

N

∫dr

∑R′

[∂kCl ′

nkφl ′]∗

e−ik·(R′−r)

× [Hk − Enk]∑

R

[∂kCl

nkφl]eik·(R−r)

= − ie

2h

[∂kCl ′

nk

]∗ 1

N

∫dr

∑R′

φ∗l ′e

−ik·R′

× [H − Enk]∑

R

φl eik·R[∂kCl

nk]

= − ie

2h

[∂kCl ′

nk

]∗ × [Hl ′l − EnkSl ′l ][∂kCl

nk

], (D3)

where Hl ′l = 〈βl ′ |H |βl〉 and Sl ′l = 〈βl ′ |βl〉. Next for the crossterm:

m(X )nk = e

hIm〈B| × [Hk − Enk]|A〉

= e

hIm

{1

N

∫dr

∑R′

[∂kCl ′

nkφl ′]∗

e−ik·(R′−r)

× [Hk − Enk]∑

R

[Cl

nkφl]eik·(R−r)i(R − r)

}

= − e

meIm

[∂kCl ′

nk

]∗ × �l ′l[Cl

nk

], (D4)

where �l ′l = 〈βl ′ |π|βl〉 and π = p + h4mec2 (σ × ∇V ). One

needs to show that the expression below vanishes:∫dr

∑R′

[∂kCl ′

nkφl ′]∗

e−ik·(R′−r)

×[Hk − Enk]∑

R

[Cl

nkφl]eik·(R−r)R =

∑R

w(R) = 0,

(D5)

or show that w(R) = −w(−R), where

w(R) =∫

dr∑

R′

[∂kCl ′

nkφl ′ (r − R′)]∗

e−ik·(R′−r)

× [Hk − Enk][Cl

nkφl (r − R)]eik·(R−r)R. (D6)

So we prove as follows:

w(−R) = −∫

dr∑

R′

[∂kCl ′

nkφl ′]∗

e−ik·(R′−r)

× [Hk − Enk][Cl

nkφl (r + R)]eik·(−R−r)R

= −∫

dr∑

R′+2R

[∂kCl ′

nkφl ′ (r + 2R − 2R − R′)]∗

× e−ik·(R′+2R−2R−r)

× [Hk − Enk][Cl

nkφl (r + 2R − R)]eik·(R−2R−r)R

= −∫

d (r + 2R)∑R′′

[∂kCl ′

nkφl ′ (r + 2R − R′′)]∗

× e−ik·(R′′−2R−r)

× [Hk − Enk][Cl

nkφl (r + 2R − R)]eik·(R−2R−r)R

= −∫

dr′ ∑R′′

[∂kCl ′

nkφl ′ (r′ − R′′)]∗

e−ik·(R′′−r′ )

× [Hk − Enk][Cl

nkφl (r′ − R)]eik·(R−r′ )R

= −w(R), (D7)

where we have replaced R′′ = R′ + 2R and r′ = r + 2R.Next, using [H, r] = −ihπ/me and (Hk − Enk )ψnk = 0, wearrive at Eq. (D4).

Finally, for the atomic term, the R and R′ in the expressionbelow can be removed using a similar procedure as for thecross term, and the final expression is simple:

m(A)nk = − ie

2h〈A| × [Hk − Enk]|A〉

= − ie

2h

1

N

∫dr

∑R′

[Cl ′

nkφl ′]∗

[−i(R′ − r)]e−ik·(R′−r)

× [Hk − Enk]∑

R

[Cl

nkφl]eik·(R−r)i(R − r)

= − e

2me

[Cl ′

nk

]∗Ll ′lC

lnk, (D8)

where Ll ′l = 〈βl ′ |r × π|βl〉.

033256-10

VALLEY ZEEMAN EFFECT AND LANDAU LEVELS IN … PHYSICAL REVIEW RESEARCH 2, 033256 (2020)

[1] D. Xiao, G.-B. Liu, W. Feng, X. Xu, and W. Yao, Phys. Rev.Lett. 108, 196802 (2012).

[2] M. Koperski, M. R. Molas, A. Aroro, K. Nogajewski, A. O.Slobodeniuk, C. Faugeras, and M. Potemski, Nanophotonics 6,1289 (2017).

[3] H. Yu, X. Cui, X. Xu, and W. Yao, Natl. Sci. Rev. 2, 57 (2015).[4] T. Mueller and E. Malic, NPJ 2D Mater. Appl. 2, 29 (2018).[5] G. Wang, A. Chernikov, M. M. Glazov, T. F. Heinz, X. Marie, T.

Amand, and B. Urbaszek, Rev. Mod. Phys. 90, 021001 (2018).[6] J. Schaibley, H. Yu, G. Clark, P. Rivera, J. S. Ross, K. L. Seyler,

W. Yao, and X. Xu, Nat. Rev. Mater. 1, 16055 (2016).[7] A. Srivastava, M. Sidler, A. V. Allain, D. S. Lembke, A. Kis,

and A. Imamoglu, Nat. Phys. 11, 141 (2015).[8] Z. Wang, J. Shan, and K. F. Mak, Nat. Nanotechnol. 12, 144

(2017).[9] W. Yao, D. Xiao, and Q. Niu, Phys. Rev. B 77, 235406 (2008).

[10] D. Xiao, M.-C. Chang, and Q. Niu, Rev. Mod. Phys. 82, 1959(2010).

[11] T. Cao, G. Wang, W. Han, H. Ye, C. Zhu, J. Shi, Q. Niu, P. Tan,E. Wang, B. Liu, and J. Feng, Nat. Commun. 3, 887 (2012).

[12] G. Wang, L. Bouet, M. M. Glazov, T. Amand, E. L. Ivchenko,E. Palleau, X. Marie, and B. Urbaszek, 2D Mater. 2, 034002(2015).

[13] M.-C. Chang and Q. Niu, Phys. Rev. B 53, 7010 (1996).[14] F. Rose, M. O. Goerbig, and F. Piéchon, Phys. Rev. B 88,

125438 (2013).[15] T. Cai, S. A. Yang, X. Li, F. Zhang, J. Shi, W. Yao, and Q. Niu,

Phys. Rev. B 88, 115140 (2013).[16] X. Li, F. Zhang, and Q. Niu, Phys. Rev. Lett. 110, 066803

(2013).[17] B. Fallahazad, H. C. P. Movva, K. Kim, S. Larentis, T.

Taniguchi, K. Watanabe, S. K. Banerjee, and E. Tutuc, Phys.Rev. Lett. 116, 086601 (2016).

[18] H. C. P. Movva, B. Fallahazad, K. Kim, S. Larentis, T.Taniguchi, K. Watanabe, S. K. Banerjee, and E. Tutuc, Phys.Rev. Lett. 118, 247701 (2017).

[19] T. Smolenski, O. Cotlet, A. Popert, P. Back, Y. Shimazaki, P.Knüppel, N. Dietler, T. Taniguchi, K. Watanabe, M. Kroner, andA. Imamoglu, Phys. Rev. Lett. 123, 097403 (2019).

[20] M. Koperski, M. R. Molas, A. Arora, K. Nogajewski, M. Bartos,J. Wyzula, D. Vaclavkova, P. Kossacki, and M. Potemski, 2DMater. 6, 015001 (2019).

[21] M. Bieniek, M. Korkusinski, L. Szulakowska, P. Potasz, I.Ozfidan, and P. Hawrylak, Phys. Rev. B 97, 085153 (2018).

[22] D. Xiao, W. Yao, and Q. Niu, Phys. Rev. lett. 99, 236809(2007).

[23] Y. Li, J. Ludwig, T. Low, A. Chernikov, X. Cui, G. Arefe, Y. D.Kim, A. M. van der Zande, A. Rigosi, H. M. Hill, S. H. Kim, J.Hone, Z. Li, D. Smirnov, and T. F. Heinz, Phys. Rev. Lett. 113,266804 (2014).

[24] D. V. Rybkovskiy, I. C. Gerber, and M. V. Durnev, Phys. Rev.B 95, 155406 (2017).

[25] A. Kormányos, P. Rakyta, and G. Burkard, New J. Phys. 17,103006 (2015).

[26] J. M. Luttinger and W. Kohn, Phys. Rev. 97, 869 (1955).[27] G.-B. Liu, W.-Y. Shan, Y. Yao, W. Yao, and D. Xiao, Phys. Rev.

B 88, 085433 (2013).

[28] J. M. Luttinger, Phys. Rev. 84, 814 (1951).[29] E. Liu, J. van Baren, T. Taniguchi, K. Watanabe, Y.-C. Chang,

and C. H. Lui, Phys. Rev. Research 1, 032007(R) (2019).[30] D. R. Hofstadter, Phys. Rev. B 14, 2239 (1976).[31] D. Ceresoli, T. Thonhauser, D. Vanderbilt, and R. Resta, Phys.

Rev. B 74, 024408 (2006).[32] N. F. Mott and H. S. W. Massey, The Theory of Atomic

Collisions (Oxford University Press, Oxford, 1965), p. 181.[33] P. Giannozzi, S. Baroni, N. Bonini, M. Calandra, R. Car, C.

Cavazzoni, D. Ceresoli, G. L. Chiarotti, M. Cococcioni, I. Daboet al., J. Phys.: Condens. Matter 21, 395502 (2009).

[34] J. P. Perdew, K. Burke, and M. Ernzerhof, Phys. Rev. Lett. 77,3865 (1996).

[35] G. Vignale and M. Rasolt, Phys. Rev. Lett. 59, 2360 (1987).[36] F. Mauri, B. G. Pfrommer, and S. G. Louie, Phys. Rev. Lett. 77,

5300 (1996).[37] M. Schlipf and F. Gygi, Comput. Phys. Commun. 196, 36

(2015).[38] M. S. Hybertsen and S. G. Louie, Phys. Rev. B 34, 5390 (1986).[39] D. Y. Qiu, F. H. da Jornada, and S. G. Louie, Phys. Rev. Lett.

111, 216805 (2013).[40] J. Deslippe, G. Samsonidze, D. A. Strubble, M. Jain, M. L.

Cohen, and S. G. Louie, Comput. Phys. Commun. 183, 1269(2012).

[41] L. Hedin, Phys. Rev. 139, A796 (1965).[42] D. Y. Qiu, F. H. da Jornada, and S. G. Louie, Phys. Rev. B 93,

235435 (2016).[43] F. H. da Jornada, D. Y. Qiu, and S. G. Louie, Phys. Rev. B 95,

035109 (2017).[44] W. Feng, Y. Yao, W. Zhu, J. Zhou, W. Yao, and D. Xiao, Phys.

Rev. B 86, 165108 (2012).[45] S. Fang, R. Kuate Defo, S. N. Shirodkar, S. Lieu, G. A. Tritsaris,

and E. Kaxiras, Phys. Rev. B 92, 205108 (2015).[46] S. A. Nikolaev and I. V. Solovyev, Phys. Rev. B 89, 064428

(2014).[47] M. Gradhand, D. V. Fedorov, F. Pientka, P. Zahn, I. Mertig, and

B. L. Györffy, J. Phys.: Condens. Matter 24, 213202 (2012).[48] Z. Li, T. Wang, C. Jin, Z. Lu, Z. Lian, Y. Meng, M. Blei, S.

Gao, T. Taniguchi, K. Watanabe, T. Ren, S. Tongay, L. Yang, D.Smirnov, T. Cao, and S.-F. Shi, Nat. Commun. 10, 2469 (2019).

[49] E. Liu, J. van Baren, Z. Lu, M. M. Altaiary, T. Taniguchi, K.Watanabe, D. Smirnov, and C. H. Lui, Phys. Rev. Lett. 123,027401 (2019).

[50] I. V. Lebedeva, D. Strubble, I. V. Tokatly, and A. Rubio, NPJComput. Mater. 5, 32 (2019).

[51] F. Xuan and S. Y. Quek (unpublished).[52] L. M. Roth, B. Lax, and S. Zwerdling, Phys. Rev. 114, 90

(1959).[53] K. L. Seyler, P. Rivera, H. Yu, N. P. Wilson, E. L. Ray, D. G.

Mandrus, J. Yan, W. Yao, and X. Xu, Nature 567, 66 (2019).[54] P. Nagler, M. V. Ballottin, A. A. Mitioglu, F. Mooshammer, N.

Paradiso, C. Strunk, R. Huber, A. Chernikov, P. C. Christianen,C. Schüller, and T. Korn, Nat. Commun. 8, 1551 (2017).

[55] T. Wozniak, P. E. Faria Junior, G. Seifert, A. Chaves, and J.Kunstmann, Phys. Rev. B 101, 235408 (2020).

[56] T. Deilmann, P. Krüger, and M. Rohlfing, Phys. Rev. Lett. 124,226402 (2020).

033256-11

Recommended